Pipeline Corrosion R&D at NIST. Richard E. Ricker Metallurgy Division Materials Performance Group Materials Science and Engineering Laboratory National Institute of Standards and Technology US Dept. of Commerce, Tech. Admin. Gaithersburg, MD 20899-8553 [email protected] Objective:.
Phases of Program
1. 1910: Congress authorized stray current corrosion study
2. 1920: Workshop convened to plan an underground corrosion study
a) Dept of Agriculture selects sites
b) Industry identifies and provide materials
c) Symposia held every 5 years
4. 1922: Ferrous pipe materials at 47 sites for 12 to 17 years
5. 1924: Other materials buried at the sites during first retrieval
6. 1928: Fe alloys, Cu, Cu alloys, and Pb samples buried at new sites
6. 1932: Materials for corrosive soils study using 15 sites (coatings)
7. 1937, 1941, 1947 materials added during retrievals at the 15 sites
8. 1945: “Underground Corrosion” by K. H. Logan NBS C450
9. 1952: Last retrival - 128 sites, >36,000 samples, 333 matl types
10. 1957: Final Rpt. “Underground Corrosion” by M. Romanoff NBS C589
11. A larger number of follow-on studies from 1957 to the present:
Ductile Cast Iron, Concentric Neutrals, Steel Pilings, Offshore Pilings, Stainless Steels, Bridge Deck Corrosion, etc.
Regression analysis for relationship of the form
The original NBS analysis determined an average k and n for each of the 47 soils. These were determine by linear regression of the equation
Log (D) = Log (k) + n Log (t)
Multiple linear regression of the k and n values as a function of soil properties met with only moderate success
Bare surface with mixing
Surface film slows transport
P=ktn n=1/2, 1/3, 1/4
Reactant consumed from environment
Therefore, the slope n is an indicator of the rate determining (limiting) process
(i) corrosion rate, and
(ii) the penetration (pitting) rate
The pitting factor (PF) is the ratio of these two rates
Analysis of the maximum pit depth data indicates that pits grow at a rate that decreases with exposure time.
For maximum pit depths, the exponent varied from about 1/4 to 1/2.
Analysis of the mass lost data indicates a higher exponent or mixed rate determining kinetics (e.g. pitting and uniform attack)
Multiple regression analysis for environmental factors influencing the exponent n has not yielded strong indicators.
Understanding the scatter in the data should help analysis.
Extreme Value Distributions
Note, one assumes that the initial scatter is due to initiation times
constant, increasing, and decreasing slopes were observed
Basic understanding of the origin of the observed scatter:
(1) Pit initiation
(2) Pit propagation
(3) Environmental variations (annual, site, irregular)
Piggable and unpiggable pipes
Laboratory Experiments designed to answer these questions
With Electrochemical Noise
EIS of Sample Cut
From Pipeline Steel
Initial Focus: Rates in environments, range of rates, and transients
Followup: Pit formation and propagation rate measurement.